The Role of Nucleation Behavior in Phase-Field Simulations of the Austenite to Ferrite Transformation M.G. MECOZZI, M. MILITZER, J. SIETSMA, and S. VAN DER ZWAAG Three-dimensional (3-D) phase-ﬁeld simulations of the austenite (c) to ferrite (a) transformation during continuous cooling at diﬀerent cooling rates were performed for an Fe-0.10C-0.49Mn (wt pct) steel, with the aim of studying the interaction between the assumed nucleation temperature range and the eﬀective interfacial mobility when ﬁtting transformation kinetics curves. Ferrite nuclei are assumed to form continuously over a temperature range of dT. An eﬀective interfacial mobility is assumed with an activation energy of 140 kJ/mol and a pre-exponential factor, l0. The pre-exponential factor and the nucleation temperature range are used as the only two adjustable parameters to match an experimental reference transformation curve for a particular cooling rate. The initial austenitic microstructure and the nuclei-density input data are based on experimental observations. A number of combinations of values (l0, dT) are found to represent the experimental reference curve equally well when related to the accuracy of experimental measurements. The comparison between the simulated and the experimental ferrite grain-size distribution is used as an additional criterion to establish the best estimate of nucleation temperature range and interface mobility. DOI: 10.1007/s11661-008-9517-2 The Author(s) 2008
NOTWITHSTANDING the continuous development of novel construction materials, the classical hotrolled C-Mn steels retain their prominent position either as a very important construction material or as input material for cold-rolled steel grades. Their properties depend on their microstructure, which itself is a function of both the steel chemistry and the thermomechanical conditions imposed during rolling, subsequent controlled cooling, and coiling. Of all the processes taking place during this ﬁnal production stage, the decomposition of the parent austenite phase into ferrite and pearlite remains of prime importance. Hence, it is not surprising that the decomposition of austenite has been modeled extensively, using a wide range of approaches. In transformation models based on the classical Johnson– Mehl–Avrami–Kolmogorov (JMAK) approach,[1–3] all attention is focused on the kinetics and all microstructural aspects are essentially ignored. However, even in the simplest JMAK model, nucleation and growth are recognized as being the two relevant and intrinsically diﬀerent M.G. MECOZZI, Graduate Student, is with the Netherlands Institute for Metals Research, 2628 CD Delft, The Netherlands, and the Department of Materials Science and Engineering, Delft University of Technology. M. MILITZER, Full Professor, is with the Center for Metallurgical Process Engineering, The University of British Columbia, Vancouver, BC, Canada V6T 1Z4. J. SIETSMA, Associate Professor, is with the Department of Materials Science and Engineering, Delft University of Technology, 2628 CD Delft, The Netherlands. Contact e-mail: [email protected]
S. VAN DER ZWAAG, Full Professor, is with the Faculty of Aerospace Engineering, Delft University of Technology, 2629 HS Delft, The Netherlands. Manuscript submitted March 7, 2007. Article published online April 4, 2008 METALLURGICAL AND MATERIALS TRANSACTIONS A
processes. When ﬁtting the JMAK equations to the experimental data, information may be obtained about both the nucleation and the growth behavior. In particular, the JMAK exponent is shown to be related to the nucleation conditions, even though only two modes of nucleation kinetics are considered: site saturation and continuous nucleation at a constant rate. In the case of site saturation, all nuclei are present and active at the start of the transformation, and their number density remains constant during the entire transformation. In the case of continuous nucleation, the number of activated nucleation sites increases at a constant rate during the transformation, with a rate of nucleus formation depending on temperature and the fraction of parent phase still present. More reﬁned transformation models do, however, incorporate relevant features of the parent microstructure. The simplest approach is that of Vandermeer, who considered the austenite grain as a sphere and the ferrite to nucleate uniformly along the outer surface. In this model, the ﬁnal ferrite grain size is necessarily identical to the prior austenite grain size, and assuming ferrite growth to be controlled by carbon diﬀusion in austenite, provides a satisfactory description of austenite decomposition in most Fe-C alloys. However, more sophisticated growth parameters (i.e., interface mobility, solute-drag eﬀect) have to be introduced as adjustable parameters to describe the growth rate of ferrite in more complex alloys, including Fe-C-Mn steels.[6–8] A geometrically more-reﬁned model is the one in which the austenite grain is assumed to be a tetrakaidecahedron. This approach allows incorporation of the ferrite nucleation site density per austenite grain as a modeling parameter to reproduce the grain size, depending on the cooling conditions. VOLUME 39A, JUNE 2008—1237
In recent years, the phase ﬁeld approach has emerged as one of the most powerful methods for modeling many types of microstructure-evolution processes, including the austenite decomposition.[10–11] Based on the construction of a Landau–Ginzburg free-energy functional, the phase-ﬁeld model treats a polycrystalline system, containing both bulk and boundary regions, in an integral manner. A set of continuous phase-ﬁeld variables, each of them representing an individual grain of the system, are deﬁned to have a constant value inside the grains and change continuously over a diﬀuse boundary of thickness g. Within this approach the initial (austenitic) microstructure is properly described, not only in two-dimensional space (2-D) but also in three-dimensional space (3-D).[12–14] Following the formation of new (ferritic) nuclei in speciﬁc locations, depending on the cooling conditions, the microstructural evolution during the austenite to ferrite transformation is governed by the phase-ﬁeld equations. The interface mobilities, interfacial energies, and the driving pressure for the transformation are parameters of the phase-ﬁeld equations, and they determine the kinetics of the austenite decomposition. The driving pressure is calculated from the local carbon composition within the diﬀuse interface, controlled by the carbon diﬀusion within the austenite. Therefore, the phase-ﬁeld model describes the ferrite growth via a mixed-mode approach, i.e., both the carbon diﬀusion and the apparent mobility of the austenite/ferrite interface are accounted for. The kinetics and diﬀusivity parameters are input data of the model, and their values have to be known for the speciﬁc material and the cooling conditions considered. The interface-energy data can be found in the literature. That is not the case for the interface mobility, which is a physically more complex parameter, which is hard to quantify with accuracy. Also, the nucleation behavior, i.e., the number of active ferrite nuclei as a function of time/temperature and their location in the initial or already partly transformed austenitic microstructure, has to be known to correctly model the austenite to ferrite transformation. The phenomenon of nucleation in solid-solid transformations has been studied extensively in the past decades,[15–17] but an accurate link between nucleation theories and phase-ﬁeld models has not been accomplished. The most important reason for this is that nucleation takes place on a length scale that is too small to incorporate in phase-ﬁeld simulations of metallic microstructures. Therefore, in the phase-ﬁeld model, the nucleation behavior has usually been implemented in a relatively simple manner, i.e., either site saturation or a constant nucleation rate is assumed.[13,14] Some experimental evidence does exist, however, (i.e., Oﬀerman et al.) that may be helpful for a better quantiﬁcation of the nucleation behavior. Not having the ambition of developing a nucleation model in its own right but to demonstrate the impact of assumptions in the nucleation conditions on the overall transformation kinetics curve and the ﬁnal grain-size distribution to develop, in the present work, we use 3-D phase-ﬁeld simulations, as presented in Militzer et al., to investigate in a controlled and systematic manner the 1238—VOLUME 39A, JUNE 2008
eﬀect of selected ferrite-nucleation parameters and of the eﬀective interface-mobility value on the ferritegrowth kinetics, and the correlation between these two parameters. The simulations are focused on the austenite to ferrite transformation kinetics, as well as on the ferritic microstructure that is to develop, but the insights to be gained apply to all diﬀusional solid-state transformations. The ferrite nuclei are set to form at diﬀerent sites, depending on the cooling conditions, while the total number of nuclei is not a ‘‘free’’ parameter but is derived from the ferrite grain size in the ﬁnal microstructure. The nucleation temperature interval and the eﬀective interface mobility are employed as the only two adjustable parameters to ﬁt a representative transformation kinetics. The most realistic combination of these two is then derived by using both the experimentally determined transformation kinetics and the ferrite grainsize distribution as comparison criteria.
The multiphase ﬁeld model derived by Steinbach et al.[10,11] is used to describe the austenite (c) to ferrite (a) transformation kinetics. In this approach, each grain is described by an appropriate order parameter, /i(r,t), with /i(r,t) = 1 if grain i is present at the location, r, and time, t, and /i(r,t) = 0 if grain i is not present at r and t. In a transition region of width gij, /i(r,t) changes continuously from 0 to 1. The interfacial thickness is taken to be the same for each pair of grains in contact, i.e., gij = g. Each grain can have a set of attributes; in the present work, only its phase, i.e., a or c, is considered, and isotropic structural and physical properties are assumed. Within this approach, the initial (austenitic) microstructure is described by a set of M phase-ﬁeld variables, /i (r,t = 0), i = 1...M, where M is the number of austenitic grains present in the initial microstructure. The formation of new (ferritic) grains, at a prescribed time, tn, is accompanied by the addition to the system of new phase-ﬁeld variables, /j(r,t), j = M + 1...M + P, where P is the number of grains imposed to form at tn. It is important to realize that the nucleation mechanism is not incorporated in the phase-ﬁeld formalism; the method requires nucleation criteria to be imposed for each individual grain. In the MICRESS program, which was used for the present study, the nucleation behavior is controlled by the value of two input parameters of the model: the ‘‘shield time’’ and the ‘‘shield distance.’’ The former is the time interval after a nucleation event within which no further nucleation can take place within a volume around the nucleus that is deﬁned by the shield distance. Thus, the shield time controls the value of the nucleation times. The shield distance is also the minimum distance between nuclei formed at the same time, thereby controlling the number and the distribution of nuclei formed at a given nucleation time. The microstructural change occurring during the austenite to ferrite transformation is described by the time evolution of N order parameters, /i(r,t), if N METALLURGICAL AND MATERIALS TRANSACTIONS A
grains, austenitic or ferritic, are present in the system. The rate of change of each order parameter, /i(r,t), is given by the pair-wise interaction between neighboring grains as follows: @/i X p2 2 2 ¼ l rij /i r /j /j r /i þ 2 /i /j j ij @t 2g ﬃﬃﬃﬃﬃﬃﬃﬃﬃ q p /i /j DGij þ ½1 g Equation  is obtained by minimising the total free energy of the system with respect to /i, under the assumption that the free-energy density is a double obstacle function of /i. When neighboring grains have diﬀerent phases, the interfacial mobilities and interfacial energies, lij and rij in Eq. , are given by the c/a interface mobility, l, and interface energy, r; DGij is the driving pressure for the transformation, i.e., DGca(x1(r,t)...xn(r,t),T), which is a function of the temperature, T, and the local composition, x1(r,t)...xn(r,t), for a system of n elements. Solute-drag eﬀects will not be taken into account in the present study, which implies that the mobility should be seen as an eﬀective mobility. When neighboring grains have the same phase (austenite or ferrite), lij and rij are the grain-boundary mobilities and energies, lcc or laa and rcc or raa, respectively. In that case, DGij is zero, and the driving pressure for grain growth is given by the respective grain-boundary energy times the curvature term (i.e., the term within the square brackets in Eq. ). Grain growth is assumed to be of secondary importance, due to the low value of the curvature term for both the c/c and a/a grain boundaries. For simplicity, grain-boundary mobilities of 5 · 10-13 m4/Js are assumed and the grain-boundary energies are set to a comparatively low value of 0.1 J/m2 to further minimize grain growth and thus facilitating that each ferrite nucleus will lead to a ferrite grain in the ﬁnal microstructures obtained in the simulations. The present work deals with the Fe-C-Mn system and the driving pressure of the c to a transformation depends on the local carbon and manganese concentration, as well as on the temperature, i.e., DG(xC(r,t), xMn(r,t), T). While in the Fe-C system, the thermodynamics are uniquely determined by the temperature and chemical composition of the system, for Fe-C-Mn, diﬀerent possible constrained equilibria may be considered for manganese. In an early work, both C and Mn were assumed to redistribute in the a and c phase. However, Mn diﬀusion was found to be extremely limited during the transformation times observed experimentally, even for cooling rates as low as 0.4 K/s. Thus, in subsequent simulations, it was assumed that interstitial carbon can redistribute between a and c by long-range diﬀusion, and that substitutional manganese does not partition during the c to a transformation (paraequilibrium). Satisfactory results were obtained with this assumption. Therefore, in the present work, the system is considered in the paraequilibrium limit; the driving pressure in Eq.  then depends on the local carbon concentration and temperature only. In the bulk of a or c phase, as well as within the diﬀuse a/a or c/c grain-boundary area, the METALLURGICAL AND MATERIALS TRANSACTIONS A
C local carbon concentration is given by xC a and xc , obtained by solving the following diﬀusion equations for the ferrite and austenite phase, respectively:
@xC C a ¼ r DC a rxa ; @t
@xC c C ¼ r DC c rxc @t
where DC k is the carbon diﬀusivity in phase k (a or c). In the diﬀuse interface between a ferritic grain, i, and an austenitic grain, j, the a and c phase coexist with a relative amount given by the phase-ﬁeld parameters, /i and /j; the local carbon concentration, xC(r,t), becomes a continuous variable in r through the interface, and it is built up from the carbon concentration in C ferrite and austenite, xC a and xc , and is given by the following equation: C xC ðr; tÞ ¼ /i ðr; tÞxC a ðr; tÞ þ /j ðr; tÞxc ðr; tÞ
Further, the diﬀusion of carbon is expressed as the sum of ﬂuxes in the ferrite and austenite phase weighted by the phase-ﬁeld parameters, /i and /j, according to the following equation: h i @xC C C C ¼ r /i DC ½4 a rxa þ ð1 /i ÞDc rxc @t In the diﬀuse interface, only phase ﬁeld parameters /i and /j are not zero and then /j = 1 - /i. A distinctive feature of the model used here is that the C xC a =xc ratio is constant within the interface, and, in the present work, is given by the following paraequilibrium ratio, kC PE: kC ¼
PE xC xC a a ¼ ¼ kC PE PE xC xC c c
Using Eqs.  and , the carbon diﬀusion Eq.  can be written as follows:
xC kC PE 1 @xC C C ¼ r D ð/i Þ rx r/ i 1 þ /i ðkC PE 1Þ @t ½6 with
DC ð/i Þ ¼
C PE C DC Da DC c þ /i k c 1 þ /i ðkC PE 1Þ
In order to calculate DGac, Thermocalc software is used to derive the binary-phase diagram in paraequilibrium condition; to accelerate the phase-ﬁeld calculations, this diagram is linearized at a reference and mFe-C are the slopes of temperature, TR. If mFe-C c a the linearized c and a line at the reference temperature R R and xC are the carbon contents at the and xC c a reference temperature, the local equilibrium temperature, Teq, corresponding to the local carbon composiand xC tion, xC c a , is calculated by the following equation: VOLUME 39A, JUNE 2008—1239
h C i CR Teq ¼ TR þ 0:5 mFeC xC xa xCR þ mFeC c c xc a a ½8 The factor 0.5 arises from the fact that the equilibrium temperature is averaged over the values calculated from the a and c line. The local undercooling is then given by the following equation: DT ¼ Teq T
The driving pressure, DGac(xC,T), in Eq.  is assumed to be proportional to the local undercooling DT, as given by the following equation: ½10 DGac xC ; T ¼ DSDT The value of DS is also evaluated using Thermocalc.
limited as veriﬁed by previous simulations. The slopes of the a/(a + c) and (a + c)/c lines, linearized at a reference temperature, TR = 1073 K, are shown in Figure 1 as dashed lines, and the carbon content in c and a at TR are reported in Table I. These data were employed for the driving-pressure calculation, according to Eq. (10), where the proportionality factor, DS, also derived using Thermocalc, is equal to 3.5 · 105 J/Km3. The equilibrium transition temperature between austenite and ferrite (Ae3 temperature), calculated from the linearized (a + c)/c line at the nominal carbon composition of 0.1 wt pct, is equal to 1106 K. Carbon diﬀusion coeﬃcients and an austenite-ferrite interfacial energy of 0.5 J/m2 were taken as described for the previous 3-D simulations. The calculations were made for a simpliﬁed 3-D austenitic grain geometry, i.e., a packing with a central tetrakaidecahedron-shaped grain, shown in Figure 2. In previous 3-D work, it was shown that the transformation kinetics are independent of the assumed initial c microstructure if the nuclei density and distribution are the same. Table II summarizes the calculation details.
Phase-ﬁeld simulations were performed to study the c to a transformation kinetics during continuous cooling in a 3-D-simulation space. The MICRESS code was used to solve numerically the phase-ﬁeld Eq.  and the carbon-diﬀusion Eq. . The simulations are performed for an Fe-0.10 wt pct C-0.49 wt pct Mn steel, for which the austenite to ferrite transformation kinetics was investigated previously using the phase-ﬁeld approach, both in 2-D and 3-D;[13,14] experimental continuouscooling transformation data are also available. Two diﬀerent cooling rates of 0.4 and 10 K/s are included in this study. Figure 1 shows the quasi-binary Fe-C phase diagram in paraequilibrium conditions, as derived by using the Thermocalc software. The assumption of paraequilibrium is probably more accurate during cooling at 10 K/s than during cooling at 0.4 K/s but is also applied here in the second case, since partitioning of manganese is very
Fig. 1—Paraequilibrium Fe-C phase diagram (dashed lines are the linearized a/(a + c) and (a + c)/c boundaries). 1240—VOLUME 39A, JUNE 2008
TR (K) 1073
Data of the Linearized Fe-C Pseudobinary Diagram under Pararequilibrium Conditions xCR a (Wt Pct)
xCR c (Wt Pct)
mFe-C a (K/Wt Pct)
mFe-C c (K/Wt Pct)
Calculation Parameters for the Initial c Microstructure
Domain Size (lm3)
Number of c Grains
dc (EQAD) (lm)
45 · 45 · 45
Fig. 2—Tetrakaidecahedron-shape initial austenite microstructure used in 3-D simulations. METALLURGICAL AND MATERIALS TRANSACTIONS A
The domain size was adjusted to have an average austenite grain size of 20 lm, equal to the value measured in metallographic cross sections of samples austenitized at 1273 K. Periodic boundary conditions are assumed in all calculations. Time stepping, mesh size, and interface thickness were varied in initial studies, and the present values were selected to obtain convergence of the numerical simulations and, at the same time, to optimize computational eﬀort. In detail, the mesh size, Dz, was set to 0.3 and 0.2 lm for the simulations at 0.4 and 10 K/s, respectively. In all simulations, the interface thickness, g, was set equal to four times the grid size, i.e., g = 4Dz, which is the defacto minimum for the interface thickness in phase-ﬁeld simulations. The nucleation parameters were deﬁned, depending on the cooling conditions. The nucleus density, q, is calculated from the measured ferrite grain size, da, using the following equation: q¼p
6 ð1:2da Þ
where fa is the ﬁnal ferrite fraction (fa = 0.9). The average ferrite grain size in 3-D is a factor 1.2 times larger than the average equivalent area diameter of ferrite grains as measured in a 2-D metallographic section. More accurately, Eq.  indicates the lower limit for the ferrite nuclei density since some ferrite coarsening may occur during transformation. Nuclei are activated in the simulations by forming a new (ferrite) grain consisting of a single volume element. At 0.4 K/s cooling rate, when the measured a grain size is approximately equal to the initial c grain size, the number of nuclei formed in the calculation domain is approximately given by the number of austenite grains. On average, for each c grain, one a nucleus is expected to form at a site with low activation energy, i.e., at an austenite grain corner. However, the employed MICRESS code does not restrict nucleation sites to grain corners. As a result, this situation is simulated by assuming that nucleation at triple lines (TLs) is the only active nucleation mode. At 10 K/s cooling rate, a substantial a grain reﬁnement is observed in the ﬁnal microstructure; the measured ferrite grain size is equal to 9 lm. This suggests that additional nucleation at less favorable sites, i.e., the grain surfaces (GSs), must become active at lower temperatures. At the lower cooling rate, the growth of earlier formed nuclei at the grain corners (TLs in the present simulation) renders the nuclei at the grain surface inactive due to carbon enrichment in austenite and the consumption of the austenite grain-boundary area. A nucleation study by Oﬀerman et al. has shown that even during very slow cooling nucleation takes place over a certain temperature range, rather than at a single value for the undercooling. Therefore, in the present simulations, the nuclei are allowed to form during cooling continuously over a nucleation temperature range, dT, the value of which cannot, however, be derived because of the conditions being distinctly diﬀerent. The infuence of the chosen value for dT METALLURGICAL AND MATERIALS TRANSACTIONS A
will be studied in combination with the value chosen for the interface mobility, a parameter that is also not known accurately. The nucleation temperature range is controlled in MICRESS by setting the value of the input-parameter shield time, i.e., the time interval after a nucleation event within which no further nucleation can take place. The number and the distribution of nuclei formed at a given temperature is controlled by the value of the shield distance, which is the radius of the zone centered in a nucleus in which nucleation is disabled. In the simulations at 0.4 K/s, the nucleation temperature range for nucleation at TLs, dTTL, is varied between 0 K (all nuclei form at a single temperature) and 24 K. In the simulation at 10 K/s, where nucleation at the GSs also occurs at lower temperatures, the total nucleation temperature range is larger compared to the case of nucleation at TLs only. A ﬁrst set of simulations at 10 K/s are run by setting all nuclei to form at GSs at a constant nucleation rate within the temperature range, dTGS, between 0 and 61 K. In a second set of simulations, the total nucleation temperature range is divided between two operational nucleation modes at TLs and at GSs, dTTL and dTGS, respectively. The number of nuclei forming at the TLs is taken to be approximately the same as for the low-cooling-rate case, and the remaining nuclei are set to form at the GSs. Table III summarizes the nucleation conditions of simulations at both cooling rates. Figure 3 shows the number of nuclei formed during cooling at 10 K/s as a function of temperature for a total-nucleation temperature range of 61 K. Due to the impossibility of evaluating the exact ferrite nucleation start temperature from experimental observations (ferrite is only recorded after a minimum fraction of approximately 1 pct is formed), the ferrite nucleation start temperature is set equal to the temperature at which ferrite is ﬁrst detected in the dilatometric tests. The a/c interface mobility, l, is assumed to be temperature dependent, according to the relation l(T) = l0 exp (-Ql/RT). In the present calculations, the activation energy, Ql, is taken to be 140 kJ/mol, the value used by Krielaart and van der Zwaag in a study on the transformation behavior of binary Fe-Mn alloys. For each employed cooling rate, l0 and dT are adjustable parameters to match a reference transformation curve, which is deﬁned based on experimental ferrite-fraction curves derived by dilatometry. The simulated ferrite-fraction curve that ﬁts the experimental one by setting all nuclei to form at a single temperature Table III.
The Nuclei Density and Resulting Average Ferrite Grain Size for Both Cooling Rates Number of Nuclei in the Domain
Cooling Rate (K/s) 0.4 10
at the TLs 15 — 17
at the GSs — 118 101
Nuclei Density, q (m-3) 14
1.7 · 10 12.9 · 1014
da (lm) 18 9
VOLUME 39A, JUNE 2008—1241
Fig. 3—Number of nuclei as a function of temperature for simulations at 10 K/s for nucleation at TLs and GSs and at GSs only, respectively, for a total-nucleation temperature interval of 61 K.
and with an adjusted mobility value is taken as the reference transformation curve.
Figure 4 shows the simulated transformation kinetics at 0.4 K/s for a ﬁxed value for l0 = 2.4 · 10-7 m4 J-1 s-1 and diﬀerent values of the temperature range for nucleation at TLs, dTTL (lines), as well as the experimental transformation curve (symbols). The maximum nucleation temperature is estimated from the experimental ferrite-fraction curve. As expected, increasing the nucleation temperature range delays the transformation for a given mobility. For the construction of Figure 4, the interface-mobility value was selected to ﬁt the experimental data when the nucleation temperature range is equal to zero (i.e., all 15 nuclei form at 1092 K), which yielded the given value of 2.4 · 10-7 m4 J-1 s-1. In this
Fig. 4—Triple-line nucleation mode at 0.4 K/s (eﬀect of nucleation temperature range, dTTL, on the transformation kinetics for a given mobility). 1242—VOLUME 39A, JUNE 2008
condition, the agreement between the experimental data and the simulation is good up to a ferrite fraction of 0.5 and when the equilibrium is reached at the ﬁnal stage of transformation. For the intermediate range of the ferrite fraction, the transformation rate is overestimated, which was observed and discussed previously. Figure 5 shows the transformation kinetics for a number of combinations of values (l0, dTTL) that ﬁt the experimental ferrite-fraction curve comparatively well and that are all within the accuracy of the experimental curve. The increase of the interface mobility is used to compensate for the increase of the nucleation temperature range in order to obtain transformation kinetics that do not diﬀer more from the previous curve than the typical experimental uncertainty. The transformation curves from the diﬀerent simulations are not identical because the eﬀects of nucleation behavior and interface mobility are more complex than a simple additivity suggests. Nevertheless, when comparing to experimental data, no signiﬁcant diﬀerence can be identiﬁed in the experimental fraction range that can be ﬁtted with high accuracy. Although phase-ﬁeld modeling also provides microstructural information, it has been chosen in the present work to use the transformation kinetics as the principal calibration curve to determine (l0, dTTL) combinations. Whereas a suitable adjustment of the apparent interfacial mobility can minimise the net eﬀect of the nucleation temperature range on the total transformation kinetics, the nucleation temperature range does have a strong eﬀect on the microstructure formed during cooling and on the ﬁnal ferrite grain size distribution. Figures 6(a) and (b) present the microstructure evolution during cooling at 0.4 K/s, with dT = 0 K. For clarity, the initial austenite microstructure is not shown in the ﬁgure. The ferrite nuclei form at the TLs simultaneously, and each grain grows approximately isotropically. The size of all 15 grains is approximately the same, leading to a narrow grain-size distribution around a mean value of 20 lm. Figures 6(c) and (d) show the microstructure evolution during cooling at 0.4 K/s for dT = 24 K. In this case, the size of each grain is related to its nucleation temperature.
Fig. 5—Triple-line nucleation mode at 0.4 K/s (change of the preexponential factor of the interface mobility at diﬀerent dTTL to have the same transformation kinetics). METALLURGICAL AND MATERIALS TRANSACTIONS A
Fig. 8—Two nucleation modes at 10 K/s (change of the pre-exponential factor of the interface mobility for diﬀerent values of dTTL and dTGS to have the same transformation kinetics).
Fig. 6—Eﬀect of dT on the simulated 3-D microstructure during cooling at 0.4 K/s for dT = 0 K (a) 1082 K and (b) 1072 K; for dT = 24 K (c) 1082 K and (d) 1072 K).
Fig. 7—Grain-surface nucleation mode at 10 K/s (change of the preexponential factor of the interface mobility for diﬀerent values of dTGS to have the same transformation kinetics).
When the last nucleus forms at 1068 K, the ﬁrst grain, nucleated at 1092 K, has a size of 27 lm, i.e., there is a signiﬁcant width in the resulting ferrite grain-size distribution. This phenomenon will be analyzed more quantitatively for the simulations at 10 K/s. Figure 7 shows the transformation kinetics at 10 K/s in a simulation in which all 118 nuclei form at the GSs. Diﬀerent combinations of l0 and the nucleation temperature range, dTGS, are selected to ﬁt the experimental ferrite-fraction curve, also reported in Figure 7. Unlike the situation for a cooling rate of 0.4 K/s, the necessary variation of l0 at 10 K/s to compensate the increase of the nucleation temperature range aﬀects the ﬁnal ferrite METALLURGICAL AND MATERIALS TRANSACTIONS A
fraction because the equilibrium cannot be reached in later transformation stages during relatively fast cooling when decreasing the interface mobility. Figure 8 shows the transformation kinetics at 10 K/s obtained by setting both TLs and GSs as activenucleation sites during transformation. Again, diﬀerent combinations of l0 and the nucleation temperature ranges, dTTL and dTGS, are chosen to obtain the same kinetics as the reference curve. Seventeen nuclei form at the TLs, approximately the same number as for the low cooling rate case, and the remaining 101 nuclei form at the GSs. Since the nucleation temperature for a given mode is assumed to be rather insensitive to the cooling rate, the ﬁrst nuclei at the TLs form again at 1092 K, similar to the low cooling rate. The remaining nuclei at the GSs form at lower temperatures. The temperature at which the ﬁrst nuclei at the GSs form is set as shown in Figure 3 such that an overlap is avoided for the temperature ranges of nucleation at TLs and at GSs, respectively. When all nuclei at the TLs are set to form at a single temperature (dTTL = 0 K), all nuclei at the GSs are assumed to form at an additional undercooling of 10 K. The values of the interface mobility used to ﬁt the reference kinetics are larger than those used in the simulations with a single nucleation mode at the GSs; this is a consequence of the initially higher nucleation rate in simulations with only nucleation at GSs (Figure 2). These results are summarized in Figure 9 where the pre-exponential factor of the interface mobility, l0, is plotted as a function of the total-nucleation temperature range, dTtotal. For a given nucleation condition, l0 increases with dTtotal.
Early publications on phase-ﬁeld modeling of the austenite to ferrite transformation showed a highly satisfactory agreement between the experimental and VOLUME 39A, JUNE 2008—1243
Fig. 9—Interface mobility as a function of the nucleation temperature spread to reproduce the reference transformation kinetics at each cooling rate.
simulated transformation kinetics when a suitable choice of the interface mobility was made.[13,23] This ability was conﬁrmed in the present work. Unlike most transformation-kinetics models, phase-ﬁeld simulations are able to reproduce the morphology of the ferrite phase produced after cooling at diﬀerent cooling rates. The major limit of these early studies was to restrict the modeling to a 2-D space. Recently, Militzer et al. reported the results of a ﬁrst series of 3-D phase-ﬁeld simulations of the austenite to ferrite transformation during continuous cooling. They showed that 3-D simulations not only describe the transformation kinetics better than 2-D simulations but also lead to a more realistic picture of the ﬁnal microstructure. In the present work, 3-D simulations oﬀer the further advantage of representing diﬀerent types of nucleation modes better than in 2-D simulations; in 2-D simulations, all nuclei form and grow in the plane of calculation while ferrite grains that appear in 2-D cuts of a simulated 3-D microstructure may be nucleated above or below the plane of view, exactly as in 2-D sections of metallographic samples. Another important aspect of selecting the nucleation sites is related to whether they are randomly distributed or occur in clusters. A homogeneous nuclei distribution in the calculation domain makes the entire domain to be homogenously transformed in agreement with the experimental microstructure, while the presence of nuclei clusters and the consequently untransformed austenite region in the ﬁnal microstructure can artiﬁcially reduce the ﬁnal ferrite fraction (Figure 10). One of the main results of the present investigation is that the eﬀective interfacial mobility required to ﬁt a given transformation curve depends strongly on the nucleation temperature range assumed: l0 increases with dT. The nucleation rate aﬀects the transformation kinetics, which explains the diﬀerent required mobilities at 10 K/s for nucleation at TLs and GSs, as compared to nucleation at GSs only (Figure 9). In order to combine both the nucleation temperature range and the nucleation rate in a single parameter, an average 1244—VOLUME 39A, JUNE 2008
Fig. 10—Eﬀect of nuclei distribution on the transformation kinetics: (a) microstructure developed with (b) a homogeneous nuclei distribution and (c) the presence of nuclei clusters.
nucleation temperature was calculated, weighting each nucleation temperature, Ti, with the number of nuclei, Ni, formed at this temperature, by following equation: P Ti Ni ½12 hTn i ¼ i Ntotal Figure 11 shows l0 as a function of the average undercooling with respect to the maximum nucleation temperature, Tn, hDTn i ¼ Tn hTn i. At 10 K/s, a single relationship was found between l0 and ÆDTnæ, independent of the operational nucleation modes. At 0.4 K/s, a much lower interface mobility is required to ﬁt the transformation. This means that the pre-exponential factor for the interface mobility depends on the cooling rate. Clearly, this is in contradiction with the physical concept of the interface migration (i.e., l0 should be METALLURGICAL AND MATERIALS TRANSACTIONS A
Fig. 11—Interface mobility as a function of the average undercooling with respect to the maximum nucleation temperature.
constant and independent of cooling rate), but this discrepancy has been observed in earlier studies on a diﬀerent steel and also for a much wider range of cooling rates. The apparent temperature dependence of l0 may be related to the solute-drag eﬀect of Mn atoms that segregate at the moving interface, as proposed by Fazeli and Militzer. In the present phaseﬁeld approach, the solute-drag term is not included in the driving-force formulation. Hence, the interface mobility, used explicitly as an adjustable parameter to ﬁt a reference kinetics in agreement with the experimental data, does not represent the intrinsic mobility of the interface, but it is an eﬀective parameter, which includes the solute-drag eﬀect. If l0 values are normalised to the value set when all nuclei form at the same temperature, i.e., hDTn i ¼ 0 K, the dependence of this normalized mobility factor on hDTn i follows the same trend for both cooling rates (Figure 12). The increase of the average nucleation undercooling, hDTn i, requires a similar relative increase of the interface mobility to reproduce the target transformation kinetics. The increase of hDTn i
Fig. 12—Normalized interface mobility as a function of the average undercooling with respect to the maximum nucleation temperature. METALLURGICAL AND MATERIALS TRANSACTIONS A
from 0 to 40 K requires an increase of l0 by a factor of 2. Due to the diﬃculty in obtaining reliable nucleation data experimentally, this eﬀect on the l0 value can be regarded as relatively small. From the preceding ﬁgures and discussion, it follows that the comparison with a given reference transformation curve does not allow establishing the correct combination of l0 and dT unambiguously and that additional data are required. The dT range can be found directly from dedicated experiments, such as the nucleation investigation of Oﬀerman et al., or indirectly from the ﬁnal ferrite grain-size distribution, as shown in this study. In order to acquire more information on the nucleation behavior, the grain-size distribution after the transformation will also be considered. Figure 13 shows the ferrite grain-size distribution obtained in simulations at 10 K/s for various dT ranges with nucleation at GSs only and two nucleation modes, respectively. The total number of 118 ferrite grains in the ﬁnal microstructure oﬀers reasonable statistics for the evaluation of the ferrite grain-size distribution. All the grain-size distributions are ﬁtted with a lognormal distribution deﬁned by the following equation: " # 1 ðln da MÞ2 pﬃﬃﬃﬃﬃﬃ exp fðda Þ ¼ ½13 2S2 da S 2p where M and S are the median value and standard deviation, respectively, of the variable ln da . The mean
Fig. 13—Simulated ferrite grain-size distributions (bars) obtained at 10 K/s with diﬀerent nucleation temperature spread for grain-surface nucleation only (left side) and triple line and grain-surface nucleation (right side) (lines show lognormal ﬁt according to Eq. ). VOLUME 39A, JUNE 2008—1245
value and the standard deviation of da, lda , and rda , respectively, are given by the following equations: Z 1 2 da fðda Þdda ¼ eMþS =2 ½14 lda ¼ 1
qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 da lda fðda Þdda ¼ e2MþS2 eS2 1 ½15
The mean value, lda , is diﬀerent from the peak value 2 ¼ eMS . The values lda and rda of the distribution, dpeak a are reported for the diﬀerent simulated grain-size distributions in Table IV. The standard deviation of the distribution depends, to a ﬁrst approximation, only on the total nucleation temperature range but not on the presence of a speciﬁc nucleation mode. The bars in Figure 14 represent the experimental ferrite grain-size distribution for the sample yielding the experimental reference kinetics curve. The 2-D grainsize values as derived from metallographic measurements are converted into 3-D grain-size values, using the
Table IV. The Mean Value and the Standard Deviation of the Ferrite Grain-Size Distributions Calculated by Fitting Lognormal Distributions dTTL dTGB dTtotal lda rda (K) (K) (K) (lm) (lm) Nucleation at GSs Nucleation at TLs and GSs
— — — 0 16 26
0 35 61 0 15 29
0 35 61 11 35 61
10.1 10.2 11.1 10.6 9.9 9.7
0.8 2.3 6.1 0.9 2.8 5.6
method proposed by Matsuura and Itoh. The lognormal ﬁt (the solid line in Figure 14) gives the values of 11.0 and 5.3 lm for the lda and rda , respectively. With these values, the simulated grain-size distribution obtained with a total temperature range of approximately 61 K ﬁts quite well with the experimental one, as shown by the dashed line in Figure 14. This result suggests that if both nucleation at TLs and grain surface occurs for a cooling rate of 10 K/s, a nucleation temperature range of approximately 30 K for each active nucleation mode may correctly reproduce the experimental grain-size distribution. At the lower cooling rate, nucleation occurs only at TLs with the temperature interval being comparable to that for nucleation at TLs as concluded for 10 K/s. The most realistic combination (l0, dT) is then determined, giving the values of l0 = 4.2 · 10-7 m4 J-1 s-1 and l0 = 29 · 10-7 m4 J-1 s-1 at 0.4 and 10 K/s, respectively.
A critical parameter study for a 3-D phase-ﬁeld model of the austenite to ferrite transformation has shown that the eﬀective interface mobility, l, and the nucleation temperature range, dT, are strongly coupled. An increase of the dT range leads to an increase of l to replicate a reference (experimental) kinetics. The analysis revealed an apparent cooling-rate dependence of l that requires further investigation, e.g., in terms of solute drag. However, the dependence of the relative mobility factor on the average undercooling for nucleation ÆDTnæ follows the same trend for both investigated cooling rates. The experimental ferrite grain-size distribution is used to establish the most realistic combination of the values for l and dT because the width of the ferrite grain-size distribution increases markedly with the nucleation temperature spread. The values of dT for each nucleation mode are estimated from the grain-size distribution, while the ﬁt of the transformation kinetics is used, together with the estimated dT, to derive the eﬀective interface mobility values for each cooling rate studied.
ACKNOWLEDGMENTS The authors thank Access for providing the MICRESS code. The authors also thank Dr. R. Huizenga for developing the software used to visualize the evolution of 3-D microstructures.
Fig. 14—Experimental ferrite grain-size distribution (bars) and lognormal ﬁt according to Eq.  (solid line). The lognormal ﬁt of the simulated grain-size distribution for a total nucleation range of 61 K is also added (dashed line). 1246—VOLUME 39A, JUNE 2008
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited. METALLURGICAL AND MATERIALS TRANSACTIONS A
REFERENCES 1. A. Kolmogorov: Izv. Akad. Nauk USSR Ser. Matemat., 1937, vol. 3, pp. 355–59. 2. W. Johnson and R. Mehl: Trans. AIME, 1939, vol. 135, pp. 416–58. 3. M. Avrami: J. Chem. Phys., 1940, vol. 8, pp. 212–24. 4. I. Tamura, C. Ouchi, T. Tanaka, and H. Sekine: Thermomechanical Processing of High Strength Low Alloy Steels, Butterworth & Co. Press, London, 1988, pp. 17–48. 5. R.A. Vandermeer: Acta Metall. Mater., 1990, vol. 38, pp. 2461–70. 6. Y. van Leeuwen, S.I. Vooijs, J. Sietsma, and S. van der Zwaag: Metall. Mater. Trans. A, 1998, vol. 29A, pp. 2925–31. 7. G.P. Krielaart and S. van der Zwaag: Mater. Sci. Technol., 1998, vol. 14, pp. 10–18. 8. T.A. Kop, Y. van Leeuwen, J. Sietsma, and S. van der Zwaag: ISIJ Int., 2000, vol. 40, pp. 713–18. 9. Y. van Leeuwen, T.A. Kop, J. Sietsma, and S. van der Zwaag: J. Phys. IV, 1999, vol. 9, pp. 401–09. 10. I. Steinbach, F. Pezzolla, B. Nestler, M. Seebelberg, R. Prieler, G.J. Schmitz, and J.L.L. Rezende: Physica D, 1996, vol. 94, pp. 135–47. 11. J. Tiaden, B. Nestler, H.J. Diepers, and I. Steinbach: Physica D, 1998, vol. 115, pp. 73–86. 12. G. Pariser, P. Shaﬀnit, I. Steinbach, and W. Bleck: Steel Res., 2001, vol. 72, pp. 354–60. 13. M.G. Mecozzi, J. Sietsma, S. van der Zwaag, M. Apel, P. Schaﬀnit, and I. Steinbach: Metall. Mater. Trans. A, 2005, vol. 36A, pp. 2327–40.
METALLURGICAL AND MATERIALS TRANSACTIONS A
14. M. Militzer, M.G. Mecozzi, J. Sietsma, and S. van der Zwaag: Acta Mater., 2006, vol. 54, pp. 3961–72. 15. H.I. Aaronson, H.A. Domian, and G.M. Pound: Trans. TMSAIME, 1966, vol. 236, pp. 753–67. 16. H.I. Aaronson, H.A. Domian, and G.M. Pound: Trans. TMSAIME, 1966, vol. 236, pp. 768–80. 17. W.C. Johnson, C.L. White, P.E. Marth, P.K. Ruf, S.M. Tuominen, K.D. Wade, K.C. Russell, and H.I. Aaronson: Metall. Trans. A, 1975, vol. 6A, pp. 911–19. 18. S.E. Oﬀerman, N.H. van Dijk, J. Sietsma, S. Grigull, E.M. Lauridsen, L. Margulies, H.F. Poulsen, M.Th. Rekveldt, and S. van der Zwaag: Science, 2002, vol. 298, pp. 1003–05. 19. B. Sundman, B. Jansson, and J.-O. Andersson: Calphad, 1985, vol. 9, pp. 153–90. 20. MICRESS software, ACCESS, Aachen, Germany, 2004. 21. A. Giumelli, M. Militzer, and E.B. Hambolt: ISIJ Int., 1999, vol. 29, pp. 271–80. 22. G.P. Krielaart and S. van der Zwaag: Mater. Sci. Technol., 1998, vol. 14, pp. 10–18. 23. Y. van Leeuwen, M. Onink, J. Sietsma, and S. van der Zwaag: ISIJ Int., 2001, vol. 41, pp. 1037–46. 24. M.G. Mecozzi, J. Sietsma, and S. van der Zwaag: Acta Mater., 2005, vol. 53, pp. 1431–40. 25. F. Fazeli and M. Militzer: Metall. Mater. Trans. A, 2005, vol. 36A, pp. 1395–1405. 26. S.K. Kurtz and F.M.A. Carpay: J. Appl. Phys., 1980, vol. 51, pp. 5725–44. 27. K. Matsuura and Y. Itoh: Mater. Trans. JIM, 1991, vol. 32, p. 1042.
VOLUME 39A, JUNE 2008—1247